Ever been told that experience is what you get when you don't get what you were expecting? How true, especially when equipment or simple oversights in preparation have led builders to waste valuable production assembly time chasing a problem. It is through experience though that we learn what we can do with confidence. The experience gained becomes gratifying once we have pinpointed the specific cause and, as a result, makes us wiser, takes less time to resolve the next time it happens, and can help others through technical forums like the one hosted by TCRA and others for the transmission rebuilders.
While the list is exponentially larger than what we have room for here, we'll explore three very common equipment and piston assembly issues, methodologies of resolution and if there are any tools that can help your shop return to production speed sooner:
Uniform contact pressure on a lockup piston during surface prep, bond and in application during lockup or controlled slip is dependent upon multiple tools and surfaces aligning parallel to one another. Beginning with fixture flatness and parallel relationship of the top to bottom fixture, the easiest way to confirm both is with a simple solder test conducted at startup with heating elements at room temperature.
|Figure 1A||Figure 1B||Figure 1C||Figure 1D|
These fixtures yielded the following measurements near the outer and inner edges:
Measurements indicate that the fixtures are parallel within 0.011", and the O.D. to I.D. flatness indicates fixtures are flat from inner to outer edges. From these measurements, we have verified that the current fixture arrangement and orientation will provide less contact pressure between the 8 o'clock and 12 o'clock positions. As a result, the clear decision is to re-machine both surfaces flat and repeat the solder test. Maximum variation should not exceed 0.007" around the fixture.
You also can use carbon transfer paper across the face of the fixture to identify any low/high points as a starting point for locating solder. Again, make sure heating elements are cold and fixtures/components are at room temperature.
Contact paper is more reliable and costs a little more; it also is a good tool to aid in identifying contact loading between the back of the piston being bonded and the fixture, as well as the relationship of the front of piston to the fixture (with and without material). Contact paper is available in multiple ranges depending on pressures being used. (For reference, I've used Pressurex, with pressure range 70 to 350 psi, from Sensor Products, LLC, Sensor Products, Inc., 300 Madison Ave., Madison, NJ 07940, 973-884-1755.)
A bond station is only as good as its maintenance history reflects and it will do what you program it to do with relatively good accuracy; however, it will only provide feedback from what it is capable of controlling. A perfect example is temperature correlation. Let's say the operator has the machine set at 450°F for both upper and lower fixtures. We could say the thermocouple-to-station-setting relationship will yield similar data. Let's bolt on a steel fixture. Now, measure the temperature of the fixture nearest the edge either supporting the piston or clamping against the friction material on the bond side. You may be surprised to find out the temperatures at the fixture are an average of 20° to 50°F lower than the bond station temperature controller. Combine this with a cover having a lot of mass, and actual bond interface temperature is now much lower than you are expecting.
Station Setting (450°F)
Temperature Near the Heating Element (445°F)
Temperature Near Piston Interface w/Probe (413°F)
Temperature Near Piston Interface w/Laser (328°F)
As long as you know the difference between actual fixture temperatures and setting temperature, you can create an offset by raising control setting temperature until actual fixture temperature matches desired temperature.
EXAMPLE: Let's say the fixture is stabilized at 425°F and the controller setting is 450°F. You will get fixture temperature close to desired temperature by adjusting controller temperature to 475°F. This is not always a proportional relationship, but close. As a result, temperature settings and correlation can become part of the routine maintenance cycle.
Taking it a step further, data loggers are available for less than $200 which plug directly into a laptop. The two-wire J-type thermocouple can be placed directly at the bondline between the adhesive and bond surface to document time/temperature curves. (Note: Either wiping adhesive completely off the test ring with MEK or placing tape over the adhesive in the area the thermocouple will be located will make it easier to remove once the cycle has finished). The software that comes with the data logger will plot your T/T curve, and you can export the data to an Excel document for graphing results of multiple settings, confirming repeatability of setups, and reviewing temperature impact on piston/cover configurations.
The plot in Figure 7 indicates that this is a typical 2-minute bond cycle, steel core/piston temperature reached 350°F in 15 seconds from room temperature, and it reached optimum cure temperature of 400°F in 32 seconds with the remaining time in the cure zone and a peak cycle temperature of 448°F. (Information gained from OE converter products supports the idea that a high-temperature fixture surface will not inhibit material integrity. For example, cottons normally found in what we know as Tan on-off lockup linings won’t burn off until 662°F.)
It goes without saying that the bigger the mass, the longer it will take to heat up and stabilize. Another key consideration is whether the component being bonded to is aluminum or steel. If it is aluminum, you can bet it will pull a lot of heat from the fixtures. In other words, fixture temps may be at 475°F before the cycle, but they may drop to 400° F or 425°F during the cycle, and it will then take longer for fixture temps to recover before bonding the next part.
Root Causing Bond Strength Issues
Here are a few questions to ask yourself if you are experiencing irregular bond issues:
Is it occurring across the entire part? If so, troubleshoot using these guidelines:
Is the issue occurring in one only section of each part?
This will identify whether the issue lies in the part or station tooling.
|Figure 8||Figure 9|
Is the problem occurring on just the O.D. or just the I.D.?
Is the piston intentionally tapered inward from O.D. to I.D.? Since some pistons like the GM 258mm are formed with a taper having an O.D. to I.D. difference of up to 0.012" (0.30 mm), it is critical to confirm the tooling matches the contour of the part (Figure 9).
A typical scenario is one in which the bond surface is machined flat and the assumption is the bottom side is parallel, when in reality, it is a formed part with the same taper on both sides (Figure 10). If both upper and lower tools are flat, the result will be a good I.D. bond and a poor O.D. bond. The I.D. is resting on the lower fixture, and as the top fixture presses down against the material, the I.D. receives full contact, BUT because of a cantilever action/deflection on the O.D., and because the actual piston is thinner here, it is not fully supported and is only receiving temperature and light contact pressure (Figure 11). Correction: Make tooling that specifically fits profile of part (Figure 12).
|Figure 10||Figure 11||Figure 12|
Intermittent bond issue, where there are alternating good and bad bond sections every X number of degrees?
When we are faced with a problem, here are a couple of closing tips to consider:
The next time you think you have a problem, ask yourself who it affects, whether you can fix it and how it compares to the problems of the less fortunate. Turns out, our converter assembly problems are just inconveniences which lead us to gain experience when we don’t get what we were expecting.
Chris Horbach is a Raybestos® product development engineer and technical advisor who writes on issues of interest to torque converter rebuilders. Raybestos® supports the Torque Converter Rebuilders Association. Learn more about the group at www.tcraonline.com. Sonnax thanks Raybestos® for allowing us to share this information with rebuilders.
While Sonnax makes every effort to ensure the accuracy of technical articles at time of publication, we assume no liability for inaccuracies or for information which may become outdated or obsolete over time.